Langmuir 2005, 21, 6366-6372
Oxygen Plasma-Treatment Effects on Si Transfer Bryan A. Langowski and Kathryn E. Uhrich* Department of Chemistry and Chemical Biology, Rutgers University, Piscataway, New Jersey 08854 Received December 23, 2004. In Final Form: March 29, 2005 Oxygen plasma-treatment is commonly used to increase the hydrophilicity of poly(dimethylsiloxane) (PDMS) stamps used for microcontact printing (µCP) aqueous-based inks. Review of the literature reveals that a wide range of plasma parameters are currently employed to modify stamp surfaces. However, little is known about the effect of these parameters (e.g., power, chamber pressure, duration) on the undesirable transfer of low-molecular-weight silicon-containing fragments from the stamps that commonly occurs during µCP. To study the effect of oxygen plasma-treatment on Si transfer, unpatterned PDMS stamps were treated with oxygen plasma under various conditions and used to stamp deionized water on plasmaactivated poly(methyl methacrylate) (PMMA) substrates. Once stamped, the PMMA substrates were analyzed with X-ray photoelectron spectroscopy (XPS) to quantify and characterize silicon present on the substrate surface. In addition, used PDMS stamps were analyzed with scanning electron microscopy (SEM) to observe topographical changes that occur during oxygen plasma-treatment. XPS results show that all plasma treatments studied significantly reduced the amount of Si transfer from the treated stamps during µCP as compared to untreated PDMS stamps and that the source of transfer is residual PDMS fragments not removed by oxygen plasma. SEM results show that, although the treated stamps undergo a variety of topographical changes, no correlation exists between stamp topography and extent of Si transfer from the stamps.
Introduction Microcontact printing (µCP)1,2 is a patterning technique that has been extensively used to produce well-defined, chemically specific patterns on a wide range of substrates. Its ease, cost-efficiency, and applicability to chemically different surfaces has made it an attractive alternative to other patterning methods,3-7 such as photolithography,8,9 which can be time-consuming and require specialized equipment not commonly found in a standard lab. In µCP, a patterned, elastomeric stamp is used to transfer molecules (i.e., “inks”) to a particular substrate, much like a regular “office stamp”, except that the raised features of the stamp have micrometer-sized dimensions. The raised portions of the stamp (i.e., the stamp pattern) are formed by casting an elastomeric polymer, most often poly(dimethylsiloxane) (PDMS), over a photolithographically fashioned mold or master. Stamps are incubated or inked with a solution of the molecules to be stamped, ultimately producing a pattern of molecules that is identical to the stamp pattern. Although µCP was initially used to pattern inorganic substrates (e.g., gold,10-12 silver,10 silicon,13 glass,13) with * Author to whom correspondence should be addressed. E-mail: [email protected]
(1) Kumar, A.; Whitesides, G. M. Appl. Phys. Lett. 1993, 63, 20022004. (2) Xia, Y.; Whitesides, G. M. Angew. Chem., Int. Ed. 1998, 37, 550575. (3) Amro, N. A.; Xu, S.; Liu, G. Langmuir 2000, 16, 3006-3009. (4) Ito, Y.; Nogawa, M. Biomaterials 2003, 24, 3021-3026. (5) Kenseth, J. R.; Harnisch, J. A.; Jones, V. W.; Porter, M. D. Langmuir 2001, 17, 4105-4112. (6) Wadu-Mesthrige, K.; Xu, S.; Amro, N. A.; Liu, G. Langmuir 1999, 15, 8580-8583. (7) Ward, J. H.; Bashir, R.; Peppas, N. A. J. Biomed. Mater. Res. 2001, 56, 351-360. (8) Schmalenberg, K. E.; Thompson, D. M.; Buettner, H. M.; Uhrich, K. E.; Garfias, L. F. Langmuir 2002, 18, 8593-8600. (9) Shin, D.-S.; Lee, K.-N.; Jang, K.-H.; Kim, J.-K.; Chung, W.-J.; Kim, Y.-K.; Lee, Y.-S. Biosens. Bioelectron. 2003, 19, 485-494. (10) Huck, W. T. S.; Yan, L.; Stroock, A.; Haag, R.; Whitesides, G. M. Langmuir 1999, 15, 6862-6867.
organic-based inks (e.g., alkylthiols,10-12 silanes,13), its range of applicability has been successfully expanded to include polymeric substrates14-24 and aqueous-based inks (e.g., proteins,14-16,18-21,23-35 RGD peptides,17 DNAsurfactant arrays,22 amphiphilic comb polymers36). Pat(11) Husemann, M.; Mecerreyes, D.; Hawker, C. J.; Hedrick, J. L.; Shah, R.; Abbott, N. L. Angew. Chem., Int. Ed. 1999, 38, 647-649. (12) Larsen, N. B.; Biebuyck, H.; Delamarche, E.; Michel, B. J. Am. Chem. Soc. 1997, 119, 3017-3026. (13) Jeon, N. L.; Choi, I. S.; Whitesides, G. M.; Kim, N. Y.; Laibinis, P. E.; Harada, Y.; Finnie, K. R.; Girolami, G. S.; Nuzzo, R. G. Appl. Phys. Lett. 1999, 75, 4201-4203. (14) Csucs, G.; Ku¨nzler, T.; Feldman, K.; Robin, F.; Spencer, N. D. Langmuir 2003, 19, 6104-6109. (15) Csucs, G.; Michel, R.; Lussi, J. W.; Textor, M.; Danuser, G. Biomaterials 2003, 24, 1713-1720. (16) Lauer, L.; Klein, C.; Offenha¨usser, A. Biomaterials 2001, 22, 1925-1932. (17) Lee, K.; Kim, D. J.; Lee, Z.; Woo, S. I.; Choi, I. S. Langmuir 2004, 20, 2531-2535. (18) McDevitt, T. C.; Angello, J. C.; Whitney, M. L.; Reinecke, H.; Hauschka, S. D.; Murry, C. E.; Stayton, P. S. J. Biomed. Mater. Res. 2002, 60, 472-479. (19) Patel, N.; Bhandari, R.; Shakesheff, K. M.; Cannizzaro, S. M.; Davies, M. C.; Langer, R.; Roberts, C. J.; Tendler, S. B.; Williams, P. M. J. Biomater. Sci. Polymer Ed. 2000, 11, 319-331. (20) Schmalenberg, K. E.; Buettner, H. M.; Uhrich, K. E. Biomaterials 2004, 25, 1851-1857. (21) Vogt, A. K.; Lauer, L.; Knoll, W.; Offenha¨usser, A. Biotechnol. Prog. 2003, 19, 1562-1568. (22) Xu, C.; Taylor, P.; Ersoz, M.; Fletcher, P. D. I.; Paunov, V. N. J. Mater. Chem. 2003, 13, 3044-3048. (23) Yang, Z.; Belu, A. M.; Liebmann-Vinson, A.; Sugg, H.; Chilkoti, A. Langmuir 2000, 16, 7482-7492. (24) Yang, Z.; Chilkoti, A. Adv. Mater. 2000, 12, 413-417. (25) Branch, D. W.; Wheeler, B. C.; Brewer, G. J.; Leckband, D. E. IEEE Trans. Biomed. Eng. 2000, 47, 290-300. (26) Corey, J. M.; Feldman, E. L. Exp. Neurol. 2003, 184, S89-S96. (27) Garrison, M. D.; McDevitt, T. C.; Luginbu¨hl, R.; Giachelli, C. M.; Stayton, P.; Ratner, B. D. Ultramicroscopy 2000, 82, 193-202. (28) James, C. D.; Davis, R. C.; Kam, L.; Craighead, H. G.; Isaacson, M.; Turner, J. N.; Shain, W. Langmuir 1998, 14, 741-744. (29) James, C. D.; Davis, R.; Meyer, M.; Turner, A.; Turner, S.; Withers, G.; Kam, L.; Banker, G.; Craighead, H.; Isaacson, M.; Turner, J.; Shain, W. IEEE Trans. Biomed. Eng. 2000, 47, 17-21. (30) Kam, L.; Boxer, S. G. J. Biomed. Mater. Res. 2001, 55, 487-495. (31) Howell, S. W.; Inerowicz, H. D.; Regnier, F. E.; Reifenberger, R. Langmuir 2003, 19, 436-439.
10.1021/la046795v CCC: $30.25 © 2005 American Chemical Society Published on Web 05/25/2005
Oxygen Plasma-Treatment Effects on Si Transfer
terning of organic-based inks is relatively straightforward in that the stamps do not require pretreatment prior to inking. However, due to the hydrophobic nature of the PDMS stamps, aqueous-based inks require modification of the patterning procedure. For example, PDMS stamp surfaces are chemically treated/oxidized to increase hydrophilicity prior to inking to ensure even distribution of molecules. Although several examples are described in the literature where nonmodified stamps have been used to pattern aqueous-based inks,14-16,18,19,21,25,27 it has been claimed that oxidized stamps exhibit better protein adsorption,28,35 more efficient transfer of ligand molecules to the stamp during inking,37 and more homogeneous pattern production.34,38-41 To modify the PDMS surface properties, stamps are derivatized with polar functional groups using traditional wet chemical methods;22,39,40 however, increased PDMS hydrophilicity can be more quickly achieved by treatment with plasma,2,17,20,23,24,28-35,37,38,41 corona discharge,42-46 or UV/ozone,47 although few instances could be found in the literature of the latter two methods being used in conjunction with µCP. Plasma is commonly employed because treatment takes only a few minutes, the chemical modifications are consistent and reproducible, and no special chemicals or waste removal is needed since gaseous byproducts are removed under vacuum. Air23,24,30,33,34,37,41 and oxygen17,20,28,32,38 are the most common feed gases used for treatment, though other gases have been employed to increase PDMS hydrophilicity.48-50 Oxygen radicals formed within the plasma oxidize the PDMS surface to produce a polar, silica-like surface that is easily wettable with polar solvents.45,48,49 However, the extent of oxidation and subsequent hydrophilicity increase are largely dependent upon the specific parameters used to generate the plasma (e.g., feed gas, power, chamber pressure, duration),48-50 and results may vary among different generators despite the use of similar parameters.51,52 A review of the literature regarding stamp plasma treatment reveals that a wide range of parameters are used and frequently the plasma (32) Kaji, H.; Takii, Y.; Nishizawa, M.; Matsue, T. Biomaterials 2003, 24, 4239-4244. (33) Kam, L.; Shain, W.; Turner, J. N.; Bizios, R. Biomaterials 2001, 22, 1049-1054. (34) Runge, A. F.; Saavedra, S. S. Langmuir 2003, 19, 9418-9424. (35) St. John, P. M.; Davis, R.; Cady, N.; Czajka, J.; Batt, C. A.; Craighead, H. G. Anal. Chem. 1998, 70, 1108-1111. (36) Hyun, J.; Ma, H.; Zhang, Z.; Beebe, J., T. P.; Chilkoti, A. Adv. Mater. 2003, 15, 576-579. (37) Lahiri, J.; Ostuni, E.; Whitesides, G. M. Langmuir 1999, 15, 2055-2060. (38) Yan, L.; Huck, W. T. S.; Zhao, X.; Whitesides, G. M. Langmuir 1999, 15, 1208-1214. (39) Donzel, C.; Geissler, M.; Bernard, A.; Wolf, H.; Michel, B.; Hilborn, J.; Delamarche, E. Adv. Mater. 2001, 13, 1164-1167. (40) He, Q.; Liu, Z.; Xiao, P.; Liang, R.; He, N.; Lu, Z. Langmuir 2003, 19, 6982-6986. (41) Liang, Z.; Li, K.; Wang, Q. Langmuir 2003, 19, 5555-5558. (42) To´th, A.; Berto´ti, I.; Blazso´, M.; Ba´nhegyi, G.; Bognar, A.; Szaplonczay, P. J. Appl. Polym. Sci. 1994, 52, 1293-1307. (43) Hillborg, H.; Gedde, U. W. Polymer 1998, 39, 1991-1998. (44) Kim, J.; Chaudhury, M. K.; Owen, M. J. IEEE Trans. Dielectr. Electr. Insul. 1999, 6, 695-702. (45) Hillborg, H.; Ankner, J. F.; Gedde, U. W.; Smith, G. D.; Yasuda, H. K.; Wikstro¨m, K. Polymer 2000, 41, 6851-6863. (46) Hillborg, H.; Sandelin, M.; Gedde, U. W. Polymer 2001, 42, 73497362. (47) Glasma¨star, K.; Gold, J.; Andersson, A. S.; Sutherland, D. S.; Kasemo, B. Langmuir 2003, 19, 5475-5483. (48) Owen, M. J.; Smith, P. J. J. Adhes. Sci. Technol. 1994, 8, 10631075. (49) Fritz, J. L.; Owen, M. J. J. Adhes. 1995, 54, 33-45. (50) Olander, B.; Wirse´n, A.; Albertsson, A. J. Appl. Polym. Sci. 2003, 90, 1378-1383. (51) Liston, E. M. J. Adhes. 1989, 30, 199-218. (52) Chan, C. M.; Ko, T. M.; Hiraoka, H. Surf. Sci. Rep. 1996, 24, 1-54.
Langmuir, Vol. 21, No. 14, 2005 6367
treatment parameters are either unknown or not stated within the studies.17,20,23,24,28-38,41,53 As all of these various treatments presumably increased stamp hydrophilicity as intended, the need to investigate and optimize these individual plasma parameters during stamp treatment did not exist. However, plasma treatment may play a larger role in the quality of microcontact- printed patterns beyond providing a simple method for increasing a PDMS stamp’s wettability. For example, we observed that plasma treatment also affects the transfer of low-molecular-weight (LMW) PDMS fragments from the stamp to the substrate during the microcontact printing process.54 Although PDMS transfer has been reported during the stamping of various substrates (e.g., carboxylic acid-derivatized poly(ethylene terephthalate),23 gold,47,55 polystyrene,14 TiO2, and SiOx 47), only a few studies have made any recommendations regarding its control or elimination.47,55 Using X-ray photoelectron spectroscopy (XPS) and time-of-flight secondary ion mass spectrometry (ToF-SIMS), Graham et al. demonstrated that low-molecular-weight silicone compounds were transferred from flat, featureless (i.e., unpatterned) PDMS stamps during the stamping of selfassembled monolayers (SAMs) of dodecanethiol onto gold.55 Because transfer of PDMS-related fragments compromises the advantages of using SAM substrates to produce clean and well-defined surfaces, Graham et al. suggested a rigorous, week-long extraction procedure for the stamps prior to µCP to significantly reduce the transfer of low-molecular-weight oligomers from the PDMS stamp surface. However, since the extracted stamps were used to pattern organic-based inks and required no additional prestamping treatments, the above cleaning procedure may not suitably eliminate Si transfer from PDMS stamps used to pattern aqueous-based inks and subjected to surface modification (e.g., plasma treatment to increase hydrophilicity) prior to use. More recently, Glasma¨star et al. used XPS and ToFSIMS to measure the amount and character of PDMS transferred from both unpatterned and patterned PDMS stamps to substrates of gold, TiO2, and SiO2 during µCP with water or buffer.47 They demonstrated that UV/ozone treatment of PDMS stamps prior to µCP significantly reduced transfer of PDMS-related material to all three inorganic substrates. Although similarities exist between oxygen plasma and UV/ozone treatments, significant differences also exist such that translation of parameters between treatments is not available. Because µCP is often used to create patterns that present markedly different chemical characteristics from the unpatterned substrate surface, the transfer of PDMSrelated material from the stamp can adversely affect the chemical homogeneity of the patterned areas, which in turn, may influence their intended function. For example, when µCP is used to ink biological ligands onto biocompatible substrates for directed cell growth,15-21,25,29,30,32,33 the transfer of silicone-containing fragments may interfere with the bioactivity of the ligand pattern or the proliferation and long-term function of the overlying cells. Consequently, means to reduce silicone transfer during µCP must be investigated to maintain the chemical integrity of patterned substrates and preserve pattern function. Although plasma treatment is a common method used (53) Hyun, J.; Zhu, Y.; Liebmann-Vinson, A.; Beebe, J., T. P.; Chilkoti, A. Langmuir 2001, 17, 6358-6367. (54) Langowski, B. A.; Uhrich, K. E. Polym. Mater.: Sci. Eng. 2002, 87, 132-133. (55) Graham, D. J.; Price, D. D.; Ratner, B. D. Langmuir 2002, 18, 1518-1527.
Langmuir, Vol. 21, No. 14, 2005
Figure 1. Schematic of µCP procedure.
to increase PDMS stamp hydrophilicity, a wide range of plasma parameters are currently utilized and their effect on the transfer of PDMS-fragments is unknown. Therefore, the role of oxygen plasma treatment on silicone transfer during the µCP of poly(methyl methacrylate) (PMMA) is discussed in this paper. As previous studies47,55 have only addressed Si transfer to inorganic substrates, this study is the first to address the minimization of Si transfer on polymeric substrates. This study is further motivated by our own observation of significant Si transfer56 during our exploration of µCP as an alternative to photolithography8 for the protein-patterning of biocompatible, plasmaactivated polymeric substrates used to direct nerve cell attachment and outgrowth.20 Unpatterned PDMS stamps were treated with oxygen plasma over a range of power levels, chamber pressures, and durations most commonly employed in the literature and used to stamp plasma-activated PMMA.20 The stamped PMMA substrates were analyzed with XPS to evaluate the amount and nature of PDMS fragments transferred from the stamp during µCP. In addition, scanning electron microscopy (SEM) was utilized to analyze the surfaces of the used PDMS stamps following µCP to evaluate topographical changes induced by the specific plasma system (i.e., power, pressure, and duration) employed. Materials and Methods Substrate and Stamp Preparation. Sheets of PMMA (Goodfellow, Huntingdon, England, 0.7 mm thick, CQ grade) were cut into pieces (8 mm × 10 mm), sonicated in HPLC grade ethanol (Sigma-Aldrich, St. Louis, MO) for 10 min, and air-dried. Unpatterned PDMS stamps were made using a Sylgard 184 silicone elastomer kit (Dow Corning, Midland, MI). Elastomer base and curing agent were combined in a 10:1 ratio (w/w) after which prepolymer was placed under vacuum to remove entrained air. Thin layers of uncured elastomer (∼10 mm) were poured into Petri dishes (150 mm × 10 mm) and allowed to cure for 24 h under vacuum (-0.98 bar, room temperature). Once cured, PDMS sheets were cut with a razor blade into stamps (10 mm × 10 mm), sonicated in HPLC grade ethanol for 10 min, and air-dried. Prior to stamping, PDMS stamps were treated with oxygen plasma (parameters described below), incubated with deionized water for 15 min, dried with filtered N2, and placed into contact with oxygen plasma-treated PMMA (parameters described below) for 15 min (see Figure 1). To ensure that stamps made complete contact with substrates, PDMS stamps were placed on the PMMA substrates and pressed down with moderate, though not excessive, finger-pressure. In addition, weights (∼13 g) were placed (56) Unpublished results.
Langowski and Uhrich on top of the PDMS stamps to provide constant pressure throughout the procedure. Additional experiments that evaluated the effect of stamping pressure on Si transfer were performed (results not included); however, there was no significant difference in transfer amounts even between extremes in pressure (e.g., no additional pressure vs over-excessive finger pressure). Upon removal of stamps, PMMA substrates were analyzed with XPS to measure Si concentration (see below) on the PMMA surface. The surfaces of the used PDMS stamps were imaged with SEM to evaluate topographical changes (see below) occurring during plasma treatment and stamping. Oxygen Plasma Treatment. Stamps and substrates were treated with oxygen plasma using a March PX-250 plasma cleaning system (March Plasma, Concord, CA). Prior to substrate and stamp treatments, the plasma chamber was purged of contaminants adhering to the chamber walls by running a “cleaning cycle” of 300 W, 580 mTorr for a duration of 900 s (recommended by the manufacturer). In each stamping experiment, PMMA substrates were plasma-treated before the PDMS stamps to ensure that any Si found on PMMA could be attributed to transfer of stamp materials and not to plasma chamber contamination. All PMMA substrates were treated at 50 W, 660 mTorr for 300 s. To evaluate the effect of individual plasma parameters (e.g., power, chamber pressure, and duration) on Si transfer, stamps were subjected to treatments in which one plasma parameter was varied, keeping the other two parameters constant. Four different power settings were evaluated (50, 100, 200, 300 W), using three different chamber pressures (225, 660, 980 mTorr). When power or pressure was varied, duration was constant at 60 s. Treatment duration (10, 30, 60, 120 s) was evaluated at both 50 W, 980 mTorr and 300 W, 225 mTorr. These ranges of power, chamber pressure, and duration were chosen because they encompass the various sets of parameters that are typically encountered in the literature. One sample for each set of parameters was subsequently analyzed with XPS. In addition, Si transfer from four stamps simultaneously treated at 300 W, 225 mTorr, and 120 s was monitored with XPS to evaluate transfer variability. XPS Analysis of PMMA Substrates. Si concentration was monitored with a Kratos XSAM 800 spectrometer using unmonochromatized Mg KR radiation (8 mA, 12 kV). To enhance surface sensitivity, the angle between sample normal and analyzer was set at 75°. Pass energies of 80 and 20 eV were used for survey and narrow energy range spectra, respectively. Four substrates stamped with untreated PDMS were analyzed in addition to substrates stamped with plasma-treated PDMS. For narrow energy range spectra, peak binding energies were referenced to the hydrocarbon C 1s peak at 285.0 eV. Because of the limited spatial resolution of XPS, we are unable to evaluate the homogeneity of fragment coverage on the PMMA substrates. For example, XPS measurements cannot distinguish between relatively large pieces of PDMS on PMMA from homogeneously distributed PDMS on PMMA because XPS analyzes a 5 mm × 5 mm area. SEM Analysis of PDMS Stamps. Topographical changes on used stamp surfaces were evaluated with an Amray 1830I scanning electron microscope, using an acceleration potential of 10 kV. Prior to imaging, stamps were sputter-coated with gold and palladium using a Balzers SCD004 sputter-coater (working pressure, 0.05 mbar; working distance, 50 mm; current, 30 mA; time, 120 s).
Results XPS Results. Survey scans of untreated PMMA detected only carbon and oxygen at the polymer surface present in a 2.6:1 ratio (Table 1), which is in close agreement with the expected ratio on the basis of the repeat unit of PMMA (2.5:1). Plasma treatment introduced oxygen-containing functionalities onto the PMMA surface and increased oxygen concentration by 7.1%, lowering the C/O ratio to 1.8:1. Survey scans of plasma-treated PMMA did not show the presence of Si, indicating that the plasma chamber is free of Si-containing contaminants that are
Oxygen Plasma-Treatment Effects on Si Transfer
Langmuir, Vol. 21, No. 14, 2005 6369
Table 1. XPS Compositional Data and Si 2p Binding Energies for PMMA and PDMSsUntreated vs Oxygen Plasma-Treateda untreated PMMA oxygen plasma-treated PMMA untreated PDMS oxygen plasma-treated PDMS a
Si 2p (eV)
72.1 65.0 47.2 24.5
27.9 35.0 29.5 50.9
0.0 0.0 23.3 24.6
Values shown are atomic %.
Table 2. Surface Topographies of PDMS Stamps Used to Generate Data in Figure 2 treatment (60 s) untreated 225 mTorr, 200 W 630 mTorr, 50 W 630 mTorr, 100 W 630 mTorr, 200 W 980 mTorr, 50 W 980 mTorr, 100 W
topography at 1000× magnificationa measurable Si transfer A C,D A,C,D A,B A A,B A,B
no measurable Si transfer 225 mTorr, 50 W D 225 mTorr, 100 W C,D 225 mTorr, 300 W A,C 630 mTorr, 300 W D 980 mTorr, 200 W D 980 mTorr, 300 W D a A, smooth; B, deep cracks; C, rippled; D, rippled/shallow cracks.
Figure 3. Representative SEM images of used PDMS stamps at 1000× magnification. Figure 2. Atomic % Si measured by XPS for PMMA stamped with PDMS stamps that were oxygen plasma-treated under various conditions: (i) untreated PDMS; (ii) varied power and chamber pressure at 60 s; (iii) varied duration at 50 W, 980 mTorr and 300 W, 225 mTorr; and (iv) identically treated stamps at optimal conditions of 300 W, 225 mTorr, and 120 s. The % Si indicates the extent of transfer of PDMS-related material during µCP. In all instances of transfer, the binding energy of the Si 2p peak was consistent with untreated PDMS (∼102.6 eV). Samples with “trace” amounts of Si showed protrusions in the background signal in the Si 2s and Si 2p regions; however, signal intensities were too low for reliable quantification. Labels “1-4” denote the four distinct stamps treated under the stated conditions.
commonly deposited onto chamber walls during PDMS plasma treatment and which can be subsequently contaminate PMMA substrates during their plasma activation. Survey scans of untreated PDMS detected the presence of silicon, in addition to carbon and oxygen, with a C/O/Si ratio of 2:1.3:1, in good agreement with the expected ratio of 2:1:1. The binding energy of the Si 2p peak was 102.6 eV, which is in good agreement with published values for PDMS42,45,47,57-59 and indicates the presence of Si species doubly bound to oxygen. Plasma treatment of PDMS increased oxygen concentration by 21%, indicating significant surface oxidation. The shift in binding energy of Si 2p to 104.3 eV indicates the presence of highly oxidized silica-like species that are formed during plasma treatment. Figure 2 shows the XPS results of PMMA substrates stamped with either untreated or plasma-exposed PDMS stamps under various treatments. Significant amounts of Si (7.0-11.1%) were detected on PMMA substrates stamped with untreated PDMS stamps. The source of Si is PDMS transferred from the stamp onto PMMA during (57) Morra, M.; Occhiello, E.; Marola, R.; Garbassi, F.; Humphrey, P.; Johnson, D. J. Colloid Interface Sci. 1990, 137, 11-24. (58) Murakami, T.; Kuroda, S.; Osawa, Z. J. Colloid Interface Sci. 1998, 202, 37-44. (59) Bar, G.; Delineau, L.; Ha¨fele, A.; Whangbo, M. H. Polymer 2001, 42, 3527-3632.
µCP. The binding energy of Si 2p is consistent with that of untreated PDMS (∼102.6 eV). Analysis of Si amounts from stamps that were plasma-treated at four powers (50, 100, 200, and 300 W) and three chamber pressures (225, 630, and 980 mTorr) showed several instances of Si transfer. However, no correlation between power or chamber pressure and Si transfer were observed for 60 s treatments. The effect of treatment duration on Si transfer was evaluated with two sets of treatments: 50 W, 980 mTorr and 300 W, 225 mTorr. These treatments were used to evaluate duration with plasma systems exhibiting different chemical- and physical-modification abilities. Figure 2 shows that treatment duration does not affect Si transfer in either plasma system. Stamps simultaneously treated under identical plasma conditions exhibited variable amounts of Si transfer, ranging from 2.2 to 4.3%, thus indicating inconsistent transfer. In all cases of Si transfer from plasma-treated stamps, the Si 2p binding energy was consistent with untreated PDMS (∼102.6 eV) and not plasma-treated PDMS (∼104.3 eV). SEM Results. Stamps used to generate the data contained in Figure 2 were imaged with SEM to evaluate topographical changes caused by plasma treatment; Table 2 summarizes the results. Although the topographical features varied widely among stamps, certain features consistently appeared, allowing stamp surfaces to be grouped into four main classifications. As shown in representative images, stamp topographies consisted of extremely smooth surfaces devoid of features (Figure 3A), smooth surfaces interspersed with cracks several micrometers wide (Figure 3B), rippled surfaces (Figure 3C), and rippled surfaces with shallow indentations and sub-micrometer cracks (Figure 3D). These topographical changes are consistent with other published studies reporting PDMS cracking45,46,48,49,60 and rippling61 (60) Hettlich, H. J.; Otterbach, F.; Mittermayer, C.; Kaufmann, R.; Klee, D. Biomaterials 1991, 12, 521-524.
Langmuir, Vol. 21, No. 14, 2005
after exposure to oxygen plasma. In many cases, topographical features were not uniformly distributed and several stamps exhibited regions of differing topographies. Topographical comparisons of stamps that transferred Si onto PMMA substrates, or not, typically displayed topographies A, C, and D. However, deep cracking (topography B) was only observed on stamps that had exhibited Si transfer and was never was found on “nontransfer” stamps. Still, not every stamp exhibiting transfer showed deep cracking, implying that the extent of Si transfer is not related to the appearance of these cracks. Discussion Although µCP is a widely used patterning technique, the related disadvantage of silicone transfer during stamping has received relatively little attention in the literature. Thus far, its control and reduction have been partially addressed by only a few studies.47,55 Using XPS and ToF-SIMS, Graham et al. illustrated Si transfer from unpatterned PDMS stamps onto gold during the microcontact printing of thiol SAMs.55 They demonstrated that low-molecular-weight PDMS, if present, can easily be transferred onto the SAM, thereby compromising the advantages of using SAM substrates to create clean, welldefined surfaces. The authors suggested a rigorous precleaning procedure whereby stamps are extracted in hexanes overnight, dried, and sonicated in ethanol/water. The entire process of extraction, drying, and sonication is repeated three times, with the whole cleaning procedure taking approximately one week. A more recent study by Glasma¨star et al. investigated UV/ozone treatment as a means to reduce silicone transfer.47 The authors used XPS and ToF-SIMS to measure the amount and character of PDMS transfer from unpatterned and patterned stamps to substrates of gold, TiO2, and SiO2 during µCP with water or buffer. In addition, they explored whether UV/ozone treatment of the PDMS stamps could reduce the amount of transferred material. XPS results showed that UV/ozone treatment oxidized the stamp surface causing (1) an increase in oxygen concentration by 7% and (2) the modification of stamp surface chemistry to a state somewhere between PDMS and silica (SiO2). The authors proposed a likely mechanism for the observed reduction of PDMS transfer by UV/ozone treatment whereby reactive oxygen radicals formed by UV light have two effects on the surface of the stamp: (i) they oxidize hydrocarbon groups that could contaminate the stamped surface and (ii) they reduce the hydrogen and carbon content in the surface region and cause a larger number of Si-O bonds. This glassy, SiOxlike surface is likely to reduce the PDMS transfer to the stamped substrate. Our results indicate extensive transfer of PDMS-related materials from untreated, flat PDMS stamps (7-11 atom % Si). This range of transfer is consistent with results from the aforementioned studies by Graham et al. and Glasma¨star et al., where untreated, unextracted stamps exhibited transfer amounts up to 12 atom % Si. However, once oxygen plasma-treated, all stamps showed marked increases in hydrophilicity and significant reduction in transfer amounts that were well below the range exhibited by untreated stamps (see Figure 2). The highest amount of Si transferred onto the PMMA substrates from plasmatreated PDMS stamps (4.3 atom % Si, Figure 2) was significantly less than the amount of Si transferred from the untreated PDMS stamps, indicating that each plasma (61) Chua, D. B. H.; Ng, H. T.; Li, S. F. Y. Appl. Phys. Lett. 2000, 76, 721-723.
Langowski and Uhrich
treatment removes residual oligomers and PDMS-related fragments to some extent. Significant Si transfer was always observed when using untreated stamps; thus, it is likely that plasma treatment is partly responsible for the removal of low-molecular-weight silicone fragments from the PDMS stamp surface. We should address our early experiments, when we noted significant amounts of Si on PMMA surfaces of PMMA that were never in direct contact with PDMS. We discovered that PMMA could be contaminated with Si by simply plasma-treating the substrates immediately after plasma-treating PDMS without running an energetic cleaning cycle between stamp and substrate treatments. Plasma-treating the PDMS caused the chamber to be contaminated with Si-containing compounds that were transferred to PMMA during subsequent plasma-treatment. Moreover, the binding energy of Si 2p on the PMMA substrates was consistent with highly oxidized Si. We concluded that Si-containing compounds are removed from the PDMS surface and deposited onto the chamber walls. Thus, when we include a cleaning cycle between PDMS stamp and PMMA substrate treatments, XPS data of the PMMA substrates showed no presence of Si. For all the experiments presented in this manuscript, a cleaning cycle was performed following each plasma treatment to eliminate the transfer of volatile species in the plasma generator. Figure 2 presents several examples in which silicone transfer was eliminated, yet many examples exist where detectable transfer occurred. Furthermore, significant variability in transfer among stamps treated with identical plasma conditions is observed, illustrating an apparent inconsistency with which oxygen plasma and/or inking removes low-molecular-weight fragments from PDMS surfaces. Of the possible explanations for the variability in Si transfer amounts among identically treated stamps, we believe that the main factor is the variability in the initial concentrations of PDMS fragments on the stamp surface prior to plasma treatment. Results from Figure 2 indicate that the initial amount of fragments vary on stamps originating from the same sheet of PDMS. Therefore, the varying amounts of Si reported for plasmatreated stamps are primarily due to differences in initial PDMS fragment concentrations rather than the ability of plasma treatment to remove/oxidize silicone. With samples simultaneously treated under identical conditions, variations in plasma composition may be responsible for the differences in transfer and this heterogeneity may treat samples differently on the basis of their locations in the chamber. To address this issue, samples were placed in the same area within the chamber and subjected to plasma whose composition should be homogeneous over such a small treatment area (∼3 cm2). In addition, plasma treatment of other polymers (PE, PP, PS, PMMA) demonstrates that samples treated under the same plasma conditions but on different days are chemically modified to the same extent, thereby ruling out the possibility that variations in plasma-generator operation are responsible.56 Thus, each plasma-treatment method exhibits approximately the same ability to remove PDMS fragments. Although all treatments reduced Si transfer onto the PMMA substrates (Figure 2), none of the plasma-treatment parameters appear to be solely responsible for silicone removal. For example, both the lowest and highest powers (50 and 300 W) showed no or trace amounts of Si. In another example, high (980 mTorr) and low (225 mTorr) chamber pressures produced samples with no Si transferred. Although these results may indicate that plasma
Oxygen Plasma-Treatment Effects on Si Transfer
compositions do not differ significantly over the power and chamber pressure ranges employed, it is more likely that the relative amounts of ions and radicals within the plasma are not a factor in silicone removal and that plasma removes residual fragments predominantly by chemical reaction of oxygen radicals, rather than physical ablation by ions. Plasma, a mixture of radicals, ions, electrons, photons, and metastable species can simultaneously modify surfaces both chemically and physically.51,52,62 Studies have shown that radicals formed within plasma are primarily responsible for chemically modifying polymers by their reaction with polymer-surface functional groups, whereas ions formed within plasma are primarily responsible for physically modifying surfaces by ablation.51,52,63 Therefore, plasma having more radicals than ions would chemically modify a substrate more than plasma having a relatively higher presence of ions, which would exhibit more physical modification and relatively less chemical incorporation. Because specific plasma parameters dictate the relative amounts of radicals and ions present in plasma, the nature of plasma-induced modifications can be controlled by the chosen parameters.52,64-66 If ion bombardment was a major factor in silicone removal, higher-power/lower-pressure treatments would show consistently less Si transferred than low-power/high-pressure plasmas. Comparison of results between treatments at 50 W, 980 mTorr and 300 W, 225 mTorr, which were expected to have distinctly different ion-to-radical ratios, show no significant differences in transfer amounts, indicating that silicone removal may primarily depend on the presence of radical species and not ions. In this respect, it is likely that oxygen plasma and UV/ ozone treatments remove residual PDMS fragments by comparable mechanisms. Both UV/ozone and oxygen plasma treatments chemically modify PDMS stamp surfaces through the oxidation of Si atoms by reactive oxygen radicals to form silica-like surface layers. Additionally, both treatments have been shown to reduce silicone transfer. Therefore, the implication is that the chemical reaction of oxygen radicals contained in both treatments is primarily responsible for the removal of silicone fragments. However, since physical modification by ion bombardment is a major characteristic of plasma treatment, physical ablation of residual fragments may be occurring in our plasma systems. The relative ion concentration may not differ significantly enough over the range of powers and pressures studied for ion bombardment to be a bigger factor in fragment removal than the oxidation of fragments by radicals. In addition to unremoved PDMS fragments pre-existing on the stamp surface, other possible sources of siliconcontaining fragments exist to transfer Si during microcontact printing. It has been well established that oxygen plasma treatment oxidizes the surface of PDMS into a brittle, silica-like (SiOx) layer that is easily cracked by mechanical or thermal stresses.46,48,49 Therefore, under extremely energetic plasma treatment (i.e., high-power treatments), this fragile surface may crack during treat(62) Wheale, S. H.; Badyal, J. P. S. In Interfacial Science; Roberts, M. W., Ed.; Blackwell Science Ltd: Oxford, 1997; pp 237-255. (63) Kersten, H. In Low-temperature plasma physics; Hippler, R., Pfau, S., Schmidt, M., Schoenbach, K. H., Eds.; Wiley-VCH: Berlin, 2001; pp 113-130. (64) Martinu, L.; Wertheimer, M. R.; Klemberg-Sapieha, J. E. In Plasma deposition and treatment of polymers; Lee, W. W., d’Agostino, R., Wertheimer, M. R., Eds.; Materials Research Society: Warrendale, 1999; Vol. 544, pp 251-255. (65) Weikart, C. M.; Yasuda, H. K. J. Polym. Sci. A Polym. Chem. 2000, 38, 3028-3042. (66) Hegemann, D.; Brunner, H.; Oehr, C. Nucl. Instr. Methods Phys. Res. B 2003, 208, 281-286.
Langmuir, Vol. 21, No. 14, 2005 6371
ment or handling, and particles originating from these cracks are subsequently transferred during stamping. However, our data do not support this possibility because no correlation exists between power and Si transfer: highpower treatments did not show more transfer than lower powers. SEM results (Table 2) further illustrated the lack of correlation between extent of cracking and Si transfer. Some stamps exhibiting cracks did not show transfer, while some uncracked stamps did show transfer. In addition, the positions of Si 2p peaks on PMMA substrates were consistent with untreated PDMS (102 eV), not plasma-treated PDMS (104 eV). Had this Si originated from the silica-like layer, the presence of highly oxidized silicon species would have been observed, as well as a correlation between cracking and Si transfer. A second possible source of Si could be pre-existing oligomers diffusing from the PDMS bulk through the treated SiOx layer of PDMS following plasma treatment. Several studies on the hydrophobic recovery of dischargeexposed PDMS demonstrated that, following treatment, pre-existing low-molecular-weight PDMS fragments diffuse onto the surface, causing a gradual decrease in surface hydrophilicity over time.42,45,49 The rate of hydrophobic recovery has also been shown to increase by deliberately stressing treated PDMS surfaces, which induces cracking of the silica-like layer and facilitates the transport of unmodified fragments onto the surface.43,46 Although this scenario would explain why the Si 2p peaks positions of transferred fragments are consistent with untreated PDMS and not with plasma-treated PDMS, the lack of correlation between cracking and Si transfer is not supportive. Diffusion of low-molecular-weight siliconecontaining fragments may not occur fast enough over the course of inking and stamping for this process to be a significant silicon source rather than residual fragments not removed by plasma treatment. A third possible Si source could be fragments/oligomers produced in-situ during plasma treatment. Studies have demonstrated that discharge treatments form low-molecular-weight components in the bulk of PDMS and other silicone-containing polymers. 44,67,68 The fragments, which are formed by chain scission, would diffuse through the bulk onto the PDMS surface, just as the pre-existing oligomers diffuse (as previously described). A study by Kim et al. demonstrated that when PDMS elastomers are exposed to mild discharges, diffusion of pre-existing silicone fluid in the elastomer plays an important role in its hydrophobic recovery.68 However, the effect of preexisting silicone compounds was found to be less significant in the recovery mechanism than the migration of in-situproduced low-molecular-weight species at severe discharge levels. As the discharge becomes severe, the authors suggested that the dominant mechanism of hydrophobic recovery is the migration of the in situ produced lowmolecular-weight silicone species from the bulk.68 These results indicate that more energetic discharge treatments (i.e., higher power) favor the formation of low-molecularweight fragments within the PDMS bulk. Results from Figure 2 show examples in which PDMS stamps treated at 300 W show little or no Si transfer, indicating that the formation and subsequent diffusion of low-molecularweight PDMS fragments formed in situ is not a significant source of Si transferred to the PMMA substrates. The results contained in this study address some interesting issues regarding Si transfer during the µCP (67) Kim, J.; Chaudhury, M. K.; Owen, M. J. J. Colloid Interface Sci. 2000, 226, 231-236. (68) Kim, J.; Chaudhury, M. K.; Owen, M. J.; Orbeck, T. J. Colloid Interface Sci. 2001, 244, 200-207.
Langmuir, Vol. 21, No. 14, 2005
of aqueous-based inks. A primary goal of these experiments was to establish a single, optimized plasma treatment that consistently eliminates silicone fragments from the PDMS stamp surface without the need for additional pretreatments. However, on the basis of our results, it appears that no single set of plasma-treatment parameters reliably eliminates silicone transfer from PDMS stamps. Instead, we found that many sets of treatment parameters significantly reduce transfer, and in some instances, reduce transfer to amounts below XPS detection limits. As there are numerous instances of using untreated PDMS stamps in the patterning of aqueous-based inks in the literature, we believe that this manuscript illustrates another advantage of plasma-treating stamps prior to use and will persuade others to reevaluate their stamping procedures. The results illustrate the common occurrence of Si transfer and the complexity of its elimination, a topic that has received surprisingly little attention in the literature and should be the focus of additional research. With the variability in Si transfer, even among identically treated stamps, it is unlikely that Si transfer can be consistently eliminated solely using oxygen plasma; additional pretreatment methods are necessary to completely eliminate Si transfer. In this respect, any of the treatments evaluated would complement the pretreatment procedure suggested by Graham et al.55 to ensure maximum reduction in Si transfer. However, because no specific plasma system was significantly better at eliminating transfer, we consider the “best” set of parameters to be based on which treatments damage the PDMS stamp surface the least. Severe topographical changes to PDMS stamp surfaces (i.e., cracking or pitting) may cause inhomogeneities on the stamp pattern that may negatively impact the quality of patterns transferred by µCP. Results from Table 2 demonstrate that only one treatment (200 W, 630
Langowski and Uhrich
mTorr, 60 s) did not alter stamp topography, implying that this treatment may be better than the rest. Thus, our results should be used as a general guide for others who wish to reduce transfer of silicone fragments during µCP. Conclusions XPS was used to monitor Si amounts on plasma-activated PMMA that were stamped with unpatterned PDMS stamps treated with oxygen plasma under various plasma powers (50-300 W), chamber pressures (225-980 mTorr), and durations (10-120 s) to systematically evaluate their roles in the undesirable transfer of PDMS-related material that occurs during µCP. In addition, SEM was used to evaluate the topographical changes occurring to PDMS stamps due to plasma treatment and stamping. Our studies demonstrated all plasma-treatment methods evaluated significantly reduced the amount of siliconerelated material transferred during stamping as compared to untreated PDMS stamps. As no correlation exists between either plasma power or chamber pressure and transfer amounts, these results indicate that silicone fragments are removed from the PDMS stamp surface primarily by chemical means due to the interaction of radical species contained within oxygen plasma. Of the many possible sources of Si transferred onto PMMA surfaces, the Si source is likely pre-existing silicone fragments not removed by plasma treatment. Acknowledgment. The authors acknowledge Dr. Ted Madey, Rutgers University, for his helpful feedback during the preparation of this manuscript and financial assistance from DuPont and NIH (DE 13207-04). LA046795V